# feasibility of graphene crlh metamaterial waveguides and leaky wave antennas

TRANSCRIPT

Feasibility of graphene CRLH metamaterial waveguides and leaky wave antennasDerrick A. Chu, Philip W. C. Hon, Tatsuo Itoh, and Benjamin S. Williams Citation: Journal of Applied Physics 120, 013103 (2016); doi: 10.1063/1.4955138 View online: http://dx.doi.org/10.1063/1.4955138 View Table of Contents: http://scitation.aip.org/content/aip/journal/jap/120/1?ver=pdfcov Published by the AIP Publishing Articles you may be interested in Evaluation of the resolution of a metamaterial acoustic leaky wave antenna J. Acoust. Soc. Am. 139, 3251 (2016); 10.1121/1.4950755 Experimental realization of a variable index transmission line metamaterial as an acoustic leaky-wave antenna Appl. Phys. Lett. 102, 203508 (2013); 10.1063/1.4807280 Leaky and bound modes in terahertz metasurfaces made of transmission-line metamaterials J. Appl. Phys. 113, 033105 (2013); 10.1063/1.4776761 Active terahertz quantum-cascade composite right/left-handed metamaterial Appl. Phys. Lett. 102, 021103 (2013); 10.1063/1.4775666 Terahertz quantum-cascade laser with active leaky-wave antenna Appl. Phys. Lett. 99, 141115 (2011); 10.1063/1.3648104

Reuse of AIP Publishing content is subject to the terms at: https://publishing.aip.org/authors/rights-and-permissions. Download to IP: 134.223.116.155 On: Sat, 16 Jul 2016

00:47:32

Feasibility of graphene CRLH metamaterial waveguides and leaky waveantennas

Derrick A. Chu,1 Philip W. C. Hon,1,2 Tatsuo Itoh,1 and Benjamin S. Williams1,3,a)

1Department of Electrical Engineering, University of California, Los Angeles, California 90095, USA2NG NEXT Nanophotonics and Plasmonics Laboratory, Northrop Grumman Aerospace Systems,Redondo Beach, California 90278, USA3California NanoSystems Institute (CNSI), University of California, Los Angeles, California 90095, USA

(Received 25 March 2016; accepted 21 June 2016; published online 6 July 2016)

The feasibility of composite right/left-handed (CRLH) metamaterial waveguides based upon

graphene plasmons is demonstrated via numerical simulation. Designs are presented that operate in

the terahertz frequency range along with their various dimensions. Dispersion relations, radiative

and free-carrier losses, and free-carrier based tunability are characterized. Finally, the radiative char-

acteristics are evaluated, along with its feasibility for use as a leaky-wave antenna. While CRLH

waveguides are feasible in the terahertz range, their ultimate utility will require precise nanofabrica-

tion, and excellent quality graphene to mitigate free-carrier losses. Published by AIP Publishing.[http://dx.doi.org/10.1063/1.4955138]

I. INTRODUCTION

Graphene shows considerable promise as an optical ma-

terial in the terahertz and mid-infrared frequency ranges as a

result of the strong optical response associated with intraband

conduction of Dirac fermions. Two-dimensional plasmons in

single and multi-layer graphene structures have been exten-

sively described theoretically and via numerical simula-

tions.1–5 Furthermore, direct evidence of their existence has

been shown in the THz and mid-IR using near-field probe

techniques,6–9 as well as using infrared absorption spectros-

copy in patterned structures (micro- and nano-ribbons, discs,

dipoles, etc.) to excite dipolar modes associated with

standing-wave plasmons.10–12 For sheet carrier concentra-

tions of �1012–1013 cm�2, THz resonances can be achieved

for structures with widths of several microns;10,11 if the sizes

are reduced to tens of nanometers, resonances in the 3–12 lm

range can be obtained.12–14 By leveraging these effects, gra-

phene has been demonstrated as a THz modulator15–17 and

has been proposed for strong light-matter coupling3,12 as well

as for resonant and leaky-wave antennas (LWAs).18–21

In this paper, we explore the feasibility of graphene for

composite right/left-handed (CRLH) metamaterial waveguides

in the terahertz and far-IR frequency range (1–15 THz). The

CRLH metamaterial concept is most easily understood using

transmission-line (TL) theory. A conventional (right-handed)

transmission-line has a series inductance (LR) and a shunt ca-

pacitance (CR); by loading the line with distributed series ca-

pacitance (CL) and shunt inductance (LL), the line becomes

highly dispersive and exhibits backward wave (left-handed)

propagation.22–24 The dispersion relation of the angular fre-

quency x vs. the propagation constant b is shown for a typical

CRLH line in Fig. 1. A stopband is evident at b¼ 0, where the

band edge frequencies are given by the shunt resonance xsh

¼ ðLLCRÞ�12 and series resonance xse ¼ ðLRCLÞ�

12. If the line

is properly designed, these resonance frequencies can be made

equal so that the stopband closes; this is known as the balanced

condition. A balanced CRLH line is particularly useful for

traveling wave devices since all modes exhibit non-zero group

velocity, and the characteristic impedance of the line is inde-

pendent of frequency. One- and two-dimensional metamateri-

als have been widely explored in the microwave frequency

range and have been used to demonstrate a variety of guided-

wave devices (e.g., multi-band and enhanced bandwidth com-

ponents, power combiners/splitters, compact resonators, phase

shifters, and phased array feed lines), as well as radiating devi-

ces (e.g., 1D and 2D resonant and leaky-wave antennas).23,25

More recently, CRLH metamaterial waveguides and metasur-

faces have been demonstrated in the THz frequency range,

FIG. 1. CRLH dispersion relationship which exhibits both right- and left-

handed characteristics. A stopband exists between xsh and xse—the shunt

and series resonance frequencies, respectively. The inset shows the charac-

teristic CRLH transmission line unit cell, which contains series inductance

LR, shunt capacitance CR, series capacitance CL, and shunt inductance LL.a)Electronic mail: [email protected]

0021-8979/2016/120(1)/013103/10/$30.00 Published by AIP Publishing.120, 013103-1

JOURNAL OF APPLIED PHYSICS 120, 013103 (2016)

Reuse of AIP Publishing content is subject to the terms at: https://publishing.aip.org/authors/rights-and-permissions. Download to IP: 134.223.116.155 On: Sat, 16 Jul 2016

00:47:32

both for passive waveguides and in active devices integrated

with THz quantum-cascade laser gain material.26,27

II. DESIGN

A. Conductivity model and graphene plasmons

We begin by considering the propagation of plasmons

by infinite, unpatterned graphene sheets on a dielectric half-

space. If coupling with free-space propagating electromag-

netic waves is neglected, graphene plasmons are described

by a dispersion relation for the in-plane wavenumber q

q ¼ i e1 þ e2ð Þxr xð Þ ; (1)

where e1 and e2 are the permittivities of the two dielectric

regions, and rðxÞ is the ac sheet conductivity of the gra-

phene. Throughout this paper, we model the graphene con-

ductivity using the Drude model as given by28

r2D xð Þ ¼ e2EF

p�h2

s1� ixs

; (2)

where EF is the Fermi level, vF ¼ 106 m/s is the Fermi veloc-

ity, e is the fundamental charge, �h is the reduced Planck’s

constant, and s is the Drude momentum relaxation time. The

Fermi level is related to the sheet carrier density n by

EF ¼ �hvF

ffiffiffiffiffiffiffiffipjnj

p: (3)

Inserting the Drude conductivity into (1) gives the dispersion

relation

q xð Þ ¼ p�h2 �1 þ �2ð Þe2EF

1þ i

sx

� �x2; (4)

which exhibits the characteristic x / q1=2 behavior associ-

ated with 2D plasmons and the x / n1=4 behavior associated

with a Dirac bandstructure.2

It has been shown that the Drude model for conductivity

does an excellent job of capturing the essential behavior

of graphene plasmons, particularly when the wavenumber

q is modest compared to the Fermi wavenumber (q� EF=�hvF),29 and at sufficiently low temperatures such that

kBT � EF. Both conditions are well satisfied for the doping

levels of graphene considered here where n � 1012 cm�2

(EF � 0:13 eV). Since we will consider plasmons with fre-

quencies of at most 15 THz (�hx � 62 meV), interband tran-

sitions will be forbidden since �hx� 2EF. More accurate

conductivity expressions that include interband transitions

and comparisons with random-phase-approximation (RPA)

based models are given in Ref. 29; treatments of nonlocal

conductivity (i.e., spatial dispersion) are given in Refs. 30

and 31. It has been shown that classical local models for the

conductivity are generally accurate for graphene nanostruc-

tures larger than �20 nm.32 Our confidence in using the local

Drude conductivity is further bolstered by reports which

show that even for 60 nm wide graphene nanoribbons, use of

a nonlocal conductivity model (where conductivity rðx; qÞis a function of both frequency and wavenumber) only shifts

resonances by 5% or less for our considered carrier concen-

trations.33 For larger nanostructures at lower frequencies, the

shifts are smaller, since the in-plane wavenumbers q involved

are smaller. As a final check, we have performed a post-

computational analysis on our simulation results by using

Fourier analysis to extract the spectral power of the current

density distribution. For the frequencies and dimensions con-

sidered here, we confirmed that 95% or more of the spectral

power is at wavenumbers sufficiently small that corrections

due to spatial dispersion are a few percent or less.30,31

B. Design of CRLH waveguide

Since CRLH metamaterials are typically described using

transmission-line (TL) models, it is useful to begin our dis-

cussion by describing the fundamental lateral plasmon mode

(m¼ 0) on a microribbon of width w using a transmission

line (TL) model (e.g., as in Refs. 31 and 34). This mode is

schematically illustrated in Fig. 2(a) along with its dispersion

relation. In the low-damping limit (xs� 1), the kinetic in-

ductance of the electrons dominates the graphene imped-

ance; this can be represented by an equivalent series inductor

LR in the circuit diagram in Fig. 1. The fringing E-field

FIG. 2. Conceptual design progression

for CRLH graphene plasmonic wave-

guide along with their associated cir-

cuit models (for one unit cell) and

dispersion relations. (a) and (b) The

fundamental m¼ 0 even mode with

and without series gaps. (c) and (d)

The higher order m¼ 1 odd mode with

and without series gaps. The latter case

shown in (d) exhibits CRLH behavior

and is the basis for the designs pre-

sented here.

013103-2 Chu et al. J. Appl. Phys. 120, 013103 (2016)

Reuse of AIP Publishing content is subject to the terms at: https://publishing.aip.org/authors/rights-and-permissions. Download to IP: 134.223.116.155 On: Sat, 16 Jul 2016

00:47:32

longitudinally couples charges along the graphene ribbon

and plays the role of the shunt capacitor CR. Effective values

for these circuit elements are given in the Appendix.

In order to realize a CRLH line, a shunt inductance LL

and a series capacitance CL must be added. It is straightfor-

ward to create a distributed series capacitance by introducing

repeated gaps of size a and period p along the graphene

microribbon. This adds a high-pass characteristic to the dis-

persion relation for the m¼ 0 mode, with a cutoff frequency

equal to the series resonance xse (see Fig. 2(b)).

In microstrip implementations, the shunt inductance LL

is typically achieved using a stub and/or via to the ground

plane. At THz frequencies, such techniques are often lossy

and difficult to fabricate; furthermore, they are incompatible

with the geometry of a single graphene microribbon.

However, an effective shunt inductance arises naturally if we

consider propagation of the first higher-order lateral mode

(labeled m¼ 1) of the microribbon (also known as an edge

mode), which is associated with transverse conduction cur-

rents. This can be modeled by two transmission lines in par-

allel, coupled together by an inductance 2LL (see Fig. 2(c)).

The effective shunt resonant frequency xsh is given by the

cutoff frequency for this higher order mode, which occurs

when the width w is approximately equal to one half of the

plasmon wavelength, i.e., qðxshÞ � p=w. This approach to

obtaining LL has been used for passive and active THz

microstrip-type waveguides.26,27,35

When gaps are introduced, the dispersion of the m¼ 1

mode takes on a CRLH character, with both right-handed

and left-handed propagating characteristics. The double

transmission line model is shown in Fig. 2(d). When this line

is excited in its odd mode, the central symmetry plane acts

as a virtual ground, so that each branch is equivalent to the

circuit in Fig. 1. With proper design, one can obtain the con-

dition xse ¼ xsh, and we say, the structure is “balanced”; the

stopband closes and propagating waves exist with non-zero

group velocity even at b¼ 0.

III. RESULTS: DISPERSION CHARACTERISTICS

A. Simulation methodology

Numerical simulations were performed using a commer-

cial finite element full-wave electromagnetic solver (Ansys

HFSS). The eigenfrequency solver was applied to a single

unit cell of length p with periodic Floquet-Bloch boundary

conditions in the axial direction for a fixed propagation con-

stant b; this was used to extract the complex eigenfrequency

x ¼ x0 þ ix00. This procedure allowed the retrieval of the

dispersion relationships x0ðbÞ.The graphene is modeled as a 2D impedance boundary

condition of Zs ¼ rðx0Þ�1at the dielectric halfspace inter-

face, where the conductivity r is taken from Eq. (2).36 The

simulation space consists of a cylindrical “airbox” of 15 lm

radius surrounding the graphene microribbon. The upper

semi-cylinder has permittivity e1 (assumed to be vacuum

throughout), and the lower semi-cylinder has permittivity e2

which represents a semi-infinite substrate. For radiating

modes, it is important to suppress reflections at the transverse

airbox boundaries; this is accomplished by using a layered

impedance boundary condition. Various airbox sizes were

considered to verify that their dimensions did not affect the

complex eigenfrequency solution.

Since the conductivity of graphene is dependent on fre-

quency, an iterative approach was used to achieve a self-

consistent solution. The algorithm is as follows: first, for a

given value of b, an initial radian frequency x0 is guessed

using the lumped element circuit model; this value is used to

calculate rðx0Þ for graphene which is input into the simula-

tion, and the complex eigenfrequency xi is solved numeri-

cally for each i-th iteration. Second, the conductivity rðx0iÞis used to re-solve for the eigenfrequency xiþ1. The process

is iterated until the real part of the complex eigenfrequency

converges within 20 GHz. As verification, this method is

seen to accurately reproduce the analytic dispersion relation

for an unpatterned graphene microribbon in its fundamental

m¼ 0 mode in Fig. 3.

The imaginary part of the eigenfrequency gives informa-

tion both about Drude loss and radiative loss (for modes

within the light line (b < nx=c)). The modal quality factor

Q is obtained from the complex eigenfrequency according to

Q ¼ x0=2x00, and with knowledge of the group velocity vg

¼ dx0=db of the mode, the power loss coefficient per unit

length is given by a ¼ x0=Qvg.

However, a complication arises if the finite element

eigenfrequency solver is used to directly extract the Drude

losses because the graphene impedance is treated as fre-

quency independent during any given iteration. Essentially,

the imaginary part of the impedance is not allowed to vary

with frequency during the eigenfrequency solution process

(equivalent to finding a root in complex frequency space).

This results in the eigenfrequency solver underestimating the

Drude contribution to the losses by as much as a factor of

two (depending upon the value of b). For example, for the

m¼ 0 guided mode, the HFSS solver calculates Q ¼ xs=2,

FIG. 3. Simulated dispersion relationship for Design A CRLH structure

(m¼ 1 with series gaps) with a center frequency of 2.8 THz (red) and dimen-

sions shown. Also shown is the dispersion for the m¼ 0 plasmonic mode on

a graphene microribbon of identical width (green). Shown in the insets are

plots of the graphene charge density q at the shunt and series resonance.

Light lines (x ¼ cb=n) for vacuum (n¼ 1) and silicon (n¼ 3.41) are also

plotted in black and gray, respectively.

013103-3 Chu et al. J. Appl. Phys. 120, 013103 (2016)

00:47:32

instead of the expected Q ¼ xs that can be calculated ana-

lytically from Eq. (4). This issue is addressed in detail in

Sec. IV A via a hybrid method, where only the radiative

losses are extracted numerically, and an analytic expression

is used for the Drude losses based upon a transmission line

model.

B. Design of a baseline CRLH structure

An exemplar CRLH waveguide was designed to operate

with a center frequency of 2.8 THz, with dimensions as fol-

lows: unit cell length p¼ 2.5 lm, capacitive gap size

a¼ 100 nm, and microribbon width w¼ 4.55 lm. Design

proceeds as follows. For a given carrier density, the width wof the microribbon is chosen first to set xsh to the frequency

of choice. The circuit model is used to give a coarse estimate

(see the Appendix); the value is then refined using a 2D full-

wave simulation for a finite width ribbon. Then, gaps are

added to the design, with an initial guess for the period p and

gap size a again provided by the circuit model. Then, the

dimensions are fine tuned using full-wave simulations so that

the CRLH structure is nearly balanced (i.e., xsh ¼ xse).

For this baseline design, which we will refer to as “Design

A,” the carrier density was taken as n ¼ 3� 1013 cm�2

(EF ¼ 0:64 eV), a value which is readily experimentally

achievable. We also assumed that the graphene structure was

at the interface of a dielectric half-space between vacuum

and a lossless silicon substrate (er ¼ 11:6). This was chosen

somewhat arbitrarily, and our results should be understood to

be applicable to a variety of dielectric substrates (i.e., SiO2,

boron nitride (BN), etc.), provided the appropriate modifica-

tions are made to the dimensions, plasmon damping rates,

and substrate dielectric and free-carrier losses. Similarly,

we have neglected any coupling with optical phonon

Reststrahlen bands in the substrates;12 such coupling is neg-

ligible at THz frequencies but is important in the mid-IR

(i.e., k � 10 lm for SiO2 and BN). Unless otherwise speci-

fied, momentum relaxation time was set to be s¼ 1 ps.

However, simulations showed that provided xs > 1, the dis-

persion relation is not sensitive to the particular value of s.

The simulated dispersion relation is presented in Fig. 3 and

exhibits the characteristics shown in Fig. 1. Left-handed

propagation is exhibited between 1.8–2.8 THz. The structure

is nearly balanced; however, if closely examined, there is a

slight �20 GHz gap that remains at b¼ 0. At this point, dis-

tinct series and shunt resonance modes can be observed, and

their charge densities are shown in the inset of Fig. 3.

However, when one considers non-zero values of b, the

propagating modes are hybrids of these two basis states. For

comparison, also shown in this figure is the dispersion of the

fundamental m¼ 0 mode for a ribbon without gaps, which

exhibits the characteristic x / b1=2 behavior. As expected,

the shunt resonance frequency occurs close to the half-

wavelength condition (i.e., bðxshÞw � 0:9p for the m¼ 0

mode). The residual 20 GHz gap is likely due to the imbalan-

ces in radiative losses associated with the shunt and series

branches of the transmission line.37,38

Several factors drive the choice of p. While ideally pshould be as small as possible to obey the metamaterial

homogenization condition, in practice as long as the period

satisfies, the condition p < ð2p=qÞ=2 no higher order Bragg

scattering will contribute to propagation. The finite-sized

unit cell also gives rise to a high-pass filtering effect, where

the series capacitance and shunt inductance behave as a high

pass filter with a cutoff of xcL ¼ 1=2ffiffiffiffiffiffiffiffiffiffiffiLLCL

p, which is seen

to be approximately 1.8 THz in this design. Reducing the

unit cell size p results in a larger value of LL and CL (required

to keep xsh and xse constant) which reduces the cutoff fre-

quency. This can be used to engineer the group velocity and

leaky-wave bandwidth of the CRLH waveguide. From a

practical standpoint, reducing the unit cell is challenging,

since the series capacitance has only a logarithmic depend-

ence on the gap size a. For example, our simulations showed

that modifying Design A by reducing the period from 2.5 lm

to 1 lm requires reducing the gap size from 100 nm to

1.3 nm to maintain the balanced condition.

C. Carrier density tunability

One of the attractive features of graphene is the ability

to tune the plasmon dispersion via electrostatic gating, chem-

ical doping, or optical pumping. This property can be

exploited to tune CRLH waveguides while approximately

maintaining their balanced character. Simulated dispersion

relations for various concentrations for our Design A struc-

ture are shown in Fig. 4. Based on the graphene dispersion

relationship presented in (4), we expect a fourth root scaling

of frequency with carrier density (i.e., x / n1=4). Indeed,

this is observed where two orders of magnitude change in

carrier density shift the center frequency by approximately a

factor of three. This will prevent tuning of a single structure

into different frequency ranges—say from the THz to the

mid-IR. However, this tuning is more than sufficient to tune

a graphene structure across the leaky-wave bandwidth (i.e.,

hundreds of GHz) for a beam-scanning or phase shifter

application. For example, a phase shift of p radians can be

obtained across a single unit cell by changing the carrier den-

sity by a factor of ten. Fig. 4 shows that the balanced

FIG. 4. Dispersion relationships for Design A for various graphene carrier

densities labeled in units cm�2.

013103-4 Chu et al. J. Appl. Phys. 120, 013103 (2016)

00:47:32

condition is approximately preserved even as the carrier den-

sity is changed. Indeed, this is predicted by the analytic

transmission-line treatment given in the Appendix for which

only geometric parameters determine the balanced condition.

However, it is seen that slight unbalancing occurs as the car-

rier density is tuned, whether this is within acceptable limits

will depend upon the application.

D. Frequency scalability

Table I presents the dimensions of several CRLH wave-

guides designed for center frequencies of 2.8 THz, 5 THz,

and 12 THz—labeled designs A, B, and C, respectively.

Dispersion relations for Design A, B, and C are plotted in

Fig. 5, along with transmission line model fits obtained using

the model and parameters given in the Appendix. It is seen

that excellent agreement is obtained although the use of sev-

eral adjustable parameters is required to properly fit the nu-

merical results. Unfortunately, the q1=2 nature of graphene

dispersion means that the width w must be reduced quadrati-

cally to achieve linear increases in frequency. This is seen in

our designs, where frequency is scaled up by a factor of 4.2

from 2.8 THz (Design A) to 12 THz (Design C), requiring

the width w to be downscaled by a factor of 17, and period pby a factor of 12.5. The gap size a shrinks only by a factor of

5 from 100 nm to 19 nm; the ability to fabricate increasingly

small gaps will no doubt be a limiting factor in any attempt

to realize mid-IR CRLH designs at 20–100 THz. We do not

present such higher frequency designs here since the small

dimensions result in increasingly large corrections on the

graphene conductivity model due to spatial dispersion (i.e.,

non-local conductivity).30,31 Such effects are not readily

incorporated into the finite-element eigenfrequency simula-

tions used here.

IV. RESULTS: RADIATIVE PROPERTIES

A. Radiative and Drude losses

In principle, graphene holds the promise of high mobil-

ity and low plasmonic dissipation—however, in practice, the

plasmon damping rates depend sensitively upon the graphene

quality and substrate interactions. Furthermore, for modes

within the light line, radiative losses must also be considered.

In this section, we consider both sources of loss and the con-

sequences for CRLH graphene waveguides.

Radiative loss is calculated using the same finite ele-

ment eigenfrequency solver described previously in Sec.

III A. However, as previously discussed, the eigenfrequency

solver overestimates Drude losses. Therefore, we imple-

mented a hybrid method, where Drude losses are deliberately

suppressed within the simulation by setting s > 1 ns. As a

result, the numerically simulated quality factor contains only

radiative losses, which we label Qr. The effect of free-carrier

loss is separately estimated assuming s¼ 1 ps using the ana-

lytic expression for the Drude quality factor that is derived in

the Appendix (see (A11)). The total quality factor is then

given by Q�1 ¼ Q�1r þ Q�1

D . Both the quality factor and

power loss coefficient a are plotted for the three designs in

Fig. 6.

Several trends are evident. First, the Drude losses for

s¼ 1 ps are very large—for Design A at 2.8 THz (aD

� 1500 cm�1), which leads to short attenuation lengths

(a�1 � 6 lm). The radiative loss is of similar magnitude,

which implies a radiative efficiency of 50% or better, but fur-

ther reduces the propagation length. Second, there is a nota-

ble discontinuity of Qr at b¼ 0. This is due to the fact the

CRLH waveguide is not perfectly balanced so that at b¼ 0 a

small 20 GHz gap remains; at this point, the modes retain

their distinctive series and shunt resonance character. Only

the shunt resonance mode exhibits dipolar character and

radiates strongly, whereas the series resonance mode is quad-

rupolar and is essentially a “dark” mode with a large Qr (see

Fig. 6(a)). Away from b¼ 0, the CRLH propagating mode is

a hybrid of both series and shunt resonances, which radiates

only via its shunt dipolar component. In fact, the presence of

this residual 20 GHz gap is likely a consequence of the fact

that only the shunt-mode radiates while the series-mode is

dark; closing the gap entirely to achieve a perfect balanced

condition would require the series mode to radiate also, as

described in Refs. 37 and 38. For designs B and C at higher

frequencies, the total quality factor increases for two reasons.

First, the Drude loss contribution scales as QD / x. Second,

the radiative loss contribution also decreases for higher fre-

quencies (Qr / x2Þ since the radiating dipole moment scales

with the width w.

How realistic is s¼ 1 ps? Within the Drude model, the

momentum relaxation time is related to the dc mobility l

TABLE I. Dimensions of frequency scaled designs.

Design

Center frequency

(THz)

Periodicity

p (lm)

Width

w (lm)

Gap

a (nm)

A 2.8 2.5 4.55 100

B 5 0.8 1.42 40

C 12 0.2 0.260 19

FIG. 5. Simulated dispersion relations for the frequency scaled designs in

Table I (points), along with fits to transmission line model presented in the

Appendix. Insets are zoomed in views of dispersion near b¼ 0.

013103-5 Chu et al. J. Appl. Phys. 120, 013103 (2016)

00:47:32

according to s ¼ lEF=ev2F, so s¼ 1 ps corresponds to a mobil-

ity of 15 600 cm2/V s for n ¼ 3� 1013 cm�2. Dc mobilities

greater than 100 000 cm2/V s have been observed at low tem-

perature in suspended graphene,39 and graphene on hexagonal

boron nitride (h-BN) underlayers has demonstrated l �60 000 cm2/V s (exfoliated sample) as well as 37 000 cm2/V s

(CVD grown).40,41 When fully encapsulated in h-BN, gra-

phene was shown to have room temperature mobilities as high

as 120 000 cm2/V s at densities of 5� 1011 cm�2, and

40 000 cm2/V s at 3� 1012 cm�2, values which correspond to

effective Drude relaxation times of s � 0:8� 1 ps. Direct

measurement of plasmon damping at room temperature at

k � 10 lm has shown s � 200� 300 fs in graphene/h-BN

structures with no dependence on carrier density.8 In summary

graphene with s � 1 ps and perhaps even higher is certainly

within experimental reach; future improvements in material

quality will only help in achieving reduced losses. Values of

s � 0:1 ps are more typical of graphene on SiO2 substrates;

such material quality is not sufficient for plasmonic CRLH

waveguide operation in the THz.

B. Beam scanning

A balanced CRLH based graphene structure can be con-

sidered for a leaky-wave antenna because its ability to scan

its main beam from backwards to broadside to forwards.25,42

Leaky-wave antennas in graphene have been proposed via

various schemes that use Bragg scattering from periodic per-

turbation, such as sinusoidal modulation of the nanoribbon

width,21 or backgating to create a periodic reactance.18 This

proposed CRLH leaky-wave antenna would differ in two sig-

nificant ways. First, radiation occurs because the fundamen-

tal dispersion of the metamaterial waveguide is within the

leaky-wave region—not due to Bragg scattering. As a result,

CRLH structures can be balanced so that there is no (in

theory) or negligibly small (in practice) stopband at b¼ 0,

which enables propagating waves across the entire leaky-

wave band. Second, the radiation of our CRLH structure is

mediated through transverse dipolar currents along the gra-

phene microribbon (i.e., through the shunt inductor).

Coupling in and out of the metamaterial waveguide thereby

occurs via coupling with transverse-electric (TE) plane

waves, rather than transverse-magnetic (TM) plane waves,

as is typical for conventional surface plasmons.27

We study beam patterns from Design A using a driven

3D full-wave simulation, where a finite length (300 lm)

CRLH waveguide is excited as a LWA. We considered the

Drude relaxation time as s¼ 1 ps and s ¼ 1 (radiative

losses only).

For the purposes of simulation, a near-field excitation is

used to drive the CRLH mode, with a horizontal electrical

dipole antenna placed 0.1 lm above the first unit cell as

shown in Fig. 7(a). This is designed to excite the transverse

current flow associated with the shunt resonance component

of the CRLH mode. In practice, a CRLH LWA might be

excited by replacing the horizontal dipole with a photocon-

ductive switch for narrowband THz generation via photomix-

ing.43 Alternately, the graphene CRLH structure might be

excited using a microstrip-type waveguide—such as from a

THz quantum-cascade laser—operating in its m¼ 1 higher-

order mode.26,35 Or, incident TE plane waves can be used to

excite single or arrays of multiple CRLH waveguides.27

The CRLH structure primarily radiates into the silicon

half-space with a beam that scans from backwards to for-

wards as the frequency is changed. In practice, radiation

from the substrate could be out-coupled and directed using a

silicon hemispherical lens as is common for THz photocon-

ductive antennas. If Drude loss is neglected (as seen in Fig.

7(b)), scanning is observed in the x-z plane from 150 to

225. At 2.75 THz (near b¼ 0), the LWA radiates broadside

with a fan-like beam. A typical beam pattern in the y-z plane

is shown in Fig. 7(c). In the far-field, the electric field is

predominately linearly polarized in the /-direction (i.e.,

transverse to the LWA axis). This is consistent with our

FIG. 6. Drude, radiative, and total quality factor assuming s¼ 1 ps for (a)

Design A centered at 2.8 THz, (b) Design B centered at 5 THz, and (c)

Design C centered at 12 THz. The shaded areas correspond to the air and sil-

icon light cones. The insets plot the total and radiative power attenuation

coefficient a. The cartoon in (a) illustrates the equivalent electric current

sources for shunt and series resonances.

013103-6 Chu et al. J. Appl. Phys. 120, 013103 (2016)

00:47:32

understanding of radiation originating from the transverse

electric current dipoles associated with the shunt resonance

component of the CRLH mode. The cross polarized compo-

nent is smaller by 10 dB or more. When a Drude relaxation

time of s ¼ 1 ps is used, the attenuation length is shorter, so

the beam is broader, and scanning is much less pronounced,

from 180 to 210 (see Fig. 7(d)). This highlights the impor-

tance of high mobility graphene for leaky wave applications.

C. Effect of a backplane

We now consider the effect of a perfect electric conduc-

tor backplane placed a distance h away from the graphene

microribbon on the substrate side. There are two possible

motivations for this: radiation control and electrostatic gat-

ing. We simulate several different backplane distances husing Design A and obtain their corresponding dispersion

relationships. First, we consider h¼ 8 lm which corresponds

to approximately k=4 at 2.8 THz within silicon. At this dis-

tance, the ground plane is sufficiently far away such that

there is little interaction between it and the fringing fields of

the graphene plasmonic mode; the dispersion relation is

unaffected (see Fig. 8). The radiative quality factor is also

similar in magnitude to the case without the backplane.

However, care must be taken when adding a backplane when

the dielectric thickness is close to a quarter wavelength, as

undesirable coupling with surface waves may result.44 A

straightforward solution to suppress these parasitic modes is

to etch the dielectric slab into a ridge underneath the gra-

phene. Such a structure will prevent excitation of surface

waves, while leaving the near-field and dispersion relation

unchanged. Although not shown here, simulations show that

this scheme preserves the scanning beam behavior except

into the air side rather than the substrate.

A smaller backplane separation can be used to reduce

radiative loss as well as allow for electrostatic gating of the

graphene. As seen in Fig. 8, the presence of the backplane

FIG. 7. (a) Schematic of near-field

dipole antenna excitation scheme used

for driven mode beam simulations. (b)

Design A far-field intensity beam pat-

tern in x–z plane for five driving fre-

quencies simulated with s ¼ 1. (c)

Far-field intensity beam pattern in (c)

y–z plane at 2.75 THz and (d) x–zplane simulated with s¼ 1 ps. All

beams are normalized to unity peak

intensity.

FIG. 8. Dispersion relationship and associated radiative quality factor Qr

(inset) for Design A with an infinite groundplane distance h placed below

the graphene strips. When the groundplane is placed close at h¼ 0.2 lm,

Design A must be rebalanced; this new design is labeled Design A0.

013103-7 Chu et al. J. Appl. Phys. 120, 013103 (2016)

00:47:32

significantly changes the dispersion relation for h ¼ 1 lm as

xsh drops due to the increase in shunt capacitance CR that

results from interaction with the ground plane. For the case

of h ¼ 0:2 lm, the change is so large that a redesign is neces-

sary to “re-balance” the CRLH waveguide; the dimensions

and dispersion is shown in Fig. 8 for this “Design A0.” The

width was reduced to 1.9 lm to increase xsh back to 2.8

THz. However, since the reduction in w also reduces CL, the

gap a is reduced to 25 nm to keep xse constant. The presence

of such a close backplane effectively shorts out the radiation

of the CRLH structure via the image currents, and the radia-

tive quality factor becomes very large (Qr � 104). This con-

figuration will also allow tuning of the CRLH dispersion via

backgating of the carrier density with modest voltages, per-

haps for applications such as phase shifters or tunable reso-

nators. Comparison with recent experimental results with

similar gate dielectric thicknesses (in SiO2) suggests that

voltages on the order of 50–100 V would be required to tune

the Fermi level from the Dirac point to the values of

0.5–1 eV necessary for our designs.12,45 An alternative to

reduce the gate voltage and obviate the need for a backgate

is to use an ion-gel top-gate, which has been shown to modu-

late the Fermi level over 1 eV with a voltage swing of

<10 V.45

V. CONCLUSION

In this work, we have introduced a new design paradigm

for graphene plasmonic CRLH waveguides and presented

several designs in the terahertz frequency range. We have

also characterized free-carrier and radiative losses, leaky-

wave antenna radiation patterns, and the effects of carrier

density tuning. A transmission-line model provides qualita-

tive design guidance and quantitative agreement with numeri-

cal results with the assistance of fitting parameters. The

dimensional requirements are challenging (i.e., the 2.8 THz

design has ribbons of width 4.5 lm and gaps of 100 nm, and

the 12 THz design has ribbons of width 260 nm and gaps of

19 nm), but within what is achievable using electron-beam li-

thography. However, the primary challenges for scaling to

higher frequencies is the requirement that dimensions shrink

quadratically with frequency as dictated by the square root

dispersion relation. The gap size a is the smallest critical

dimension and will likely be the primary limiting factor for

fabrication if these structures were to be scaled up to the mid-

IR, since it would need to shrink to just a few nanometers.

The issue of loss is the most critical challenge for practi-

cal CRLH graphene devices. For example at 3 THz, for

practical values of the graphene mobility (i.e., s¼ 1 ps,

l � 15 600 cm2/V s), losses are large and propagation

lengths limited. Radiative losses are also large—this benefits

radiative efficiency for leaky-wave antennas but results in

reduced beam scanning and large beamwidths. Hence, the

most critical challenge for practical implementation is the

need for large-area high-mobility graphene to minimize plas-

mon dissipation and achieve times of s > 1 ps. For guided

wave operation, radiative losses can be eliminated with the

addition of a backplane, which can also act as a backgate for

free-carrier tuning. By tuning the carrier concentration by

one order of magnitude, 180 of phase shift can be obtained

even over the length of one unit cell—an attractive feature

for a distributed phase shifter. The situation for losses

improves somewhat at higher frequencies (i.e., 5 THz and 12

THz), since the Drude quality factor for CRLH modes scales

proportionally to x, and the radiative quality factor Qr scales

as x2 due to the quadratic reduction in waveguide dimen-

sions. These challenges are not unique to our design—

indeed, they are ubiquitous for any device based upon plas-

mons.46 However, the reduced group velocity of the CRLH

waveguide reduces the propagation length by a factor two

and the Q by a factor of �0.75 compared to an unpatterned

graphene plasmon.

In summary, our results show that while demonstrating

CRLH graphene waveguides is possible, it will be challeng-

ing, with the ultimate performance highly dependent upon

availability of high-mobility graphene with long Drude

relaxation times. This challenge will need to be weighed

against potential benefits of using graphene, such as free-

carrier tunability, or large optical nonlinearity.

ACKNOWLEDGMENTS

The authors would like to thank Ziwen Wang for his

preliminary simulation work. This research was supported in

part by National Science Foundation Grant Nos. ECCS

1150071 and ECCS 1340928.

APPENDIX: CRLH TRANSMISSION LINE MODEL

The theory of CRLH metamaterials is most easily pre-

sented in terms of a transmission-line model. In the graphene

microribbon waveguide presented here, this is not strictly

valid since the CRLH behavior is based upon a higher-order

transverse mode, which results in an approximately sinusoi-

dal variation in the electric and magnetic fields across the

width of the ribbon. Thus, the waveguide cannot be consid-

ered sub-wavelength in the transverse dimension, and the

quasi-static limit is not applicable. Nonetheless, a circuit

model is still very useful for qualitative understanding and

design guidance, provided that it is understood that induc-tances and capacitances are effective parameters. However,

for detailed design, numerical methods must be used. We

begin by defining the series inductance LR and shunt capaci-

tance CR for a graphene microribbon with an effective width

weff and unit cell length p

LR ¼ �p

weffxIm r�1f g ¼ pp�h2

weffe2EF; (A1)

CR ¼ DRpweffðe1 þ e2ÞRefqðxÞg; (A2)

¼ DRpweffp�h2 e1 þ e2ð Þ2

e2EFx2: (A3)

The series inductance LR originates from the kinetic induct-

ance of the graphene free carriers, i.e., the imaginary part of

the Drude resistivity in (2). We neglect any additional

“Faraday inductance” associated with the graphene currents,

which is negligible in the non-retarded limit (i.e., q� x=c).31

013103-8 Chu et al. J. Appl. Phys. 120, 013103 (2016)

00:47:32

The effective shunt capacitance CR was obtained by equating

the dispersion relation of a conventional transmission line b¼ x

ffiffiffiffiffiffiffiffiLRCR

p

p to the graphene plasmon dispersion relation given

in (4) for an infinite graphene sheet. This requires CR to ac-

quire a frequency/wavenumber dependence. However, an

additional factor DR has been added which enhances the ca-

pacitance to account for the modification of the dispersion due

to the finite width of the microribbon. DR can be obtained ei-

ther through matching to numerical simulations, or by using

the term g calculated in Ref. 34 (DR � ð2p2gÞ2 in which g is

evaluated at qw ¼ p). Using this expression, we accordingly

take DR¼ 1.8, 1.8, and 1.9 for Designs A, B, and C, respec-

tively. This expression for CR also neglects the effects of

quantum-capacitance, which is appropriate here where the

non-local corrections to conductivity are negligible.30,31 For

the fundamental lateral mode m¼ 0, the effective width weff is

equal to the physical ribbon width w. In this case, these

expressions are equivalent to those derived in Ref. 31, taken

in the limit that kBT � EF, and ignoring the negligible contri-

butions of quantum capacitance, and Faraday inductance.

The CRLH waveguide mode is based upon an m¼ 1

higher order lateral mode (i.e., an edge mode) and includes

series capacitive gaps of size a. We model this according to

the double transmission line circuit model shown in Fig. 2(d)

operating in its odd mode. The previous expressions for LR

and CR still apply, provided that the effective width in this

case is weff ¼ Fw=2. This reflects the fact that branch of the

TL has physical width of w=2, and the effective width is

modified by a factor F to reflect that the current, field, and

charge are nonuniform over the width of the ribbon. We can

approximate this factor as F ¼ 2=pA; ideally A¼ 1, which is

appropriate for a field distribution takes on exactly a half-

sinusoidal transverse variation.27 In reality, there is a slight

phase shift associated with the reflection of the plasmon

from the microribbon edge; we find A¼ 0.9, 0.96, and 1.0

for designs A, B, and C, respectively. We also define the

shunt inductance

LL ¼ �weff

pxIm r�1f g ¼ weffp�h2

pe2EF; (A4)

which is based upon the same kinetic inductance of the gra-

phene used to define LR, except now for a section of length

of weff and width of p. This ensures that the effective shunt

frequency xsh ¼ ðLLCRÞ�1=2corresponds the condition

where the microribbon width w is nearly equal to one-half of

the plasmon wavelength such that qðxshÞ ¼ Ap=w.

A working expression for the series capacitance CL can

be obtained from the capacitance between metal patches of

width weff and length p=2 on a dielectric half-space in the

limit that p� a (derived for a Sievenpiper surface in Ref.

47), which gives

CL ¼ DLweff

pe1 þ e2ð Þln 2p=að Þ: (A5)

DL is a phenomenological factor that is required to reduce

xse ¼ ðLRCLÞ�1=2so that it matches the simulated result. We

fit the values of DL¼ 0.7, 0.66, and 0.6 for the dimensions of

designs A, B, and C, respectively. Without this factor, CL is

overestimated since the period of the structure is not suffi-

ciently subwavelength to accurately use a lumped element

expression.

Despite the presence of the phenomenological parame-

ters, we can still draw important conclusions. For example,

by equating these analytic expressions for the series and

shunt resonance frequencies, we are able to obtain a tran-

scendental equation for the CRLH balanced condition

DL ln 2p=að Þ ¼ w

p

ffiffiffiffiffiffiDR

p

A: (A6)

This expression for the balanced condition contains only

geometric parameters; there is no dependence on carrier con-

centration or other material properties. This implies that the

balanced dispersion relation will be preserved as the carrier

density is changed, which is consistent with the tuning

observed in the numerical simulations in Fig. 4.

Drude loss within the graphene can be included by add-

ing resistances

RR ¼2pp�h2

weffe2EFs; RL ¼

2weffp�h2

pe2EFs; (A7)

in series with LR and LL, respectively. We can further use

this formalism to derive an analytic expression for loss in a

CRLH waveguide. The dispersion for a balanced line is

given25

b ¼ xp

ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiLR þ iRR=xð ÞCR

p� 1

px1ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffi

LL þ iRL=xð ÞCL

p : (A8)

This gives a power attenuation coefficient

a ¼ 2Im bf g ¼ 2

ps

ffiffiffiffiffiffiffiffiffiffiffiLRCR

pþ 2

px2s1ffiffiffiffiffiffiffiffiffiffiffi

LLCL

p : (A9)

For a balanced CRLH structure, at b¼ 0, the attenuation

coefficient is

a x ¼ xsh ¼ xseð Þ ¼4

ps

ffiffiffiffiffiffiffiffiffiffiffiLRCR

p¼ 4p�h2 e1 þ e2ð Þx

se2EF; (A10)

which is twice as large as for an unpatterned m¼ 0 graphene

plasmon mode at the same frequency. The quality factor

associated with Drude loss can then be obtained using the

relation QD ¼ x=avg; at b¼ 0, it has the value of

QD ¼ x=avg: (A11)

This relation is used to estimate the Drude losses in Fig. 6.

We note that at b¼ 0, QD ¼ ð3=4Þxs—three quarters of the

value of QD of an unpatterned m¼ 0 graphene plasmon.

1M. Jablan, H. Buljan, and M. Soljacic, Phys. Rev. B 80, 245435 (2009).2E. H. Hwang and S. Das Sarma, Phys. Rev. B 75, 205418 (2007).3F. H. L. Koppens, D. E. Chang, and F. J. Garc�ıa de Abajo, Nano Lett. 11,

3370 (2011).4A. Y. Nikitin, F. Guinea, F. J. Garc�ıa-Vidal, and L. Mart�ın-Moreno, Phys.

Rev. B 84, 161407 (2011).5A. N. Grigorenko, M. Polini, and K. S. Novoselov, Nat. Photonics 6, 749

(2012).

013103-9 Chu et al. J. Appl. Phys. 120, 013103 (2016)

00:47:32

6Z. Fei, G. O. Andreev, W. Bao, L. M. Zhang, A. S. McLeod, C. Wang,

M. K. Stewart, Z. Zhao, G. Dominguez, M. Thiemens, M. M. Fogler, M. J.

Tauber, A. H. Castro-Neto, C. N. Lau, F. Keilmann, and D. N. Basov,

Nano Lett. 11, 4701 (2011).7Z. Fei, A. S. Rodin, G. O. Andreev, W. Bao, A. S. McLeod, M. Wagner,

L. M. Zhang, Z. Zhao, M. Thiemens, G. Dominguez, M. M. Fogler, A. H.

C. Neto, C. N. Lau, F. Keilmann, and D. N. Basov, Nature 487, 82–85

(2012).8A. Woessner, M. B. Lundeberg, Y. Gao, A. Principi, P. Alonso-Gonz�alez,

M. Carrega, K. Watanabe, T. Taniguchi, G. Vignale, M. Polini, J. Hone,

R. Hillenbrand, and F. H. L. Koppens, Nat. Mater. 14, 421 (2014).9J. Chen, M. Badioli, P. Alonso-Gonz�alez, S. Thongrattanasiri, F. Huth, J.

Osmond, M. Spasenovic, A. Centeno, A. Pesquera, P. Godignon, A. Z.

Elorza, N. Camara, F. J. G. de Abajo, R. Hillenbrand, and F. H. L.

Koppens, Nature 487, 77–81 (2012).10L. Ju, B. Geng, J. Horng, C. Girit, M. Martin, Z. Hao, H. A. Bechtel, X.

Liang, A. Zettl, Y. R. Shen, and F. Wang, Nat. Nanotechnol. 6, 630

(2011).11H. Yan, X. Li, B. Chandra, G. Tulevski, Y. Wu, M. Freitag, W. Zhu, P.

Avouris, and F. Xia, Nat. Nanotechnol. 7, 330 (2012).12V. W. Brar, M. S. Jang, M. Sherrott, J. J. Lopez, and H. A. Atwater, Nano

Lett. 13, 2541 (2013).13H. Yan, T. Low, W. Zhu, Y. Wu, M. Freitag, X. Li, F. Guinea, P. Avouris,

and F. Xia, Nat. Photonics 7, 394 (2013).14X. Zhu, W. Wang, W. Yan, M. B. Larsen, P. Bøggild, T. G. Pedersen, S.

Xiao, J. Zi, and N. A. Mortensen, Nano Lett. 14, 2907 (2014).15R. Yan, B. Sensale-Rodriguez, L. Liu, D. Jena, and H. G. Xing, Opt.

Express 20, 28664 (2012).16B. Sensale-Rodriguez, R. Yan, M. M. Kelly, T. Fang, K. Tahy, W. S.

Hwang, D. Jena, L. Liu, and H. G. Xing, Nat. Commun. 3, 780 (2012).17S. H. Lee, M. Choi, T.-T. Kim, S. Lee, M. Liu, X. Yin, H. K. Choi, S. S.

Lee, C.-G. Choi, S.-Y. Choi, X. Zhang, and B. Min, Nat. Mater. 11, 936

(2012).18M. Esquius-Morote, J. S. G�omez-D�ıaz, and J. Perruisseau-Carrier, IEEE

Trans. Terahertz Sci. Technol. 4, 116 (2014).19R. Filter, M. Farhat, M. Steglich, R. Alaee, C. Rockstuhl, and F. Lederer,

Opt. Express 21, 3737 (2013).20I. Llatser, C. Kremers, A. Cabellos-Aparicio, E. A. Josep Miquel Jornet,

and D. N. Chigrin, Photonics Nanostruct.: Fundam. Appl. 10, 353 (2012).21J. S. G�omez-D�ıaz, M. Esquius-Morote, and J. Perruisseau-Carrier, Opt.

Express 21, 24856 (2013).22C. Caloz and T. Itoh, in Proceedings of the IEEE-AP-S USNC/URSI

National Radio Science Meeting (2002), Vol. 2, p. 412.23A. Lai, C. Caloz, and T. Itoh, IEEE Microwave Mag. 5, 34 (2004).24G. V. Eleftheriades, A. K. Iyer, and P. C. Kremer, IEEE Trans. Microwave

Theory Tech. 50, 2702 (2002).

25C. Caloz and T. Itoh, Electromagnetic Metamaterials: Transmission LineTheory and Microwave Applications (Wiley, 2006).

26A. A. Tavallaee, P. W. C. Hon, Q.-S. Chen, T. Itoh, and B. S. Williams,

Appl. Phys. Lett. 102, 021103 (2013).27P. W. C. Hon, Z. Liu, T. Itoh, and B. S. Williams, J. Appl. Phys. 113,

033105 (2013).28J. Horng, C.-F. Chen, B. Geng, C. Girit, Y. Zhang, Z. Hao, H. Bechtel, M.

Martin, A. Zettl, M. Crommie, Y. Shen, and F. Wang, Phys. Rev. B 83,

165113 (2011).29F. J. Garc�ıa de Abajo, ACS Photonics 1, 135 (2014).30G. Lovat, G. W. Hanson, R. Araneo, and P. Burghignoli, Phys. Rev. B 87,

115429 (2013).31D. Correas-Serrano, J. S. G�omez-D�ıaz, J. Perruisseau-Carrier, and A.

�Alvarez Melc�on, IEEE Trans. Terahertz Sci. Technol. 61, 4333 (2013).32S. Thongrattanasiri, A. Manjavacas, and F. J. Garc�ıa de Abajo, ACS Nano

6, 1766 (2012).33A. Fallahi, T. Low, M. Tamagnone, and J. Perruisseau-Carrier, Phys. Rev.

B 91, 121405(R) (2015).34J. Christensen, A. Manjavacas, S. Thongrattanasiri, F. H. L. Koppens, and

F. J. Garc�ıa de Abajo, ACS Nano 6, 431 (2012).35A. A. Tavallaee, B. S. Williams, P. W. C. Hon, T. Itoh, and Q.-S. Chen,

Appl. Phys. Lett. 99, 141115 (2011).36J. Gomez-Diaz and J. Perruisseau-Carrier, in 2012 International

Symposium on Antennas and Propagation (ISAP) (2012), pp. 239–242.37J. S. G�omez-D�ıaz, D. Canete-Rebenaque, and A. �Alvarez Melc�on, IEEE

Antennas Wireless Propag. Lett. 10, 29 (2011).38S. Otto, A. Rennings, K. Solbach, and C. Caloz, IEEE Trans. Antennas

Propag. 59, 3695 (2011).39K. I. Bolotin, K. J. Sikes, Z. Jiang, M. Klima, G. Fudenberg, J. Hone, P.

Kim, and H. L. Stormer, Solid State Commun. 146, 351 (2008).40W. Gannett, W. Regan, K. Watanabe, T. Taniguchi, M. F. Crommie, and

A. Zettl, Appl. Phys. Lett. 98, 242105 (2011).41C. R. Dean, A. F. Young, I. Meric, C. Lee, L. Wang, S. Sorgenfrei, K.

Watanabe, T. Taniguchi, P. Kim, K. L. Shepard, and J. Hone, Nat.

Nanotechnol. 5, 722 (2010).42S. Lim, C. Caloz, and T. Itoh, IEEE Trans. Microwave Theory Tech. 53,

161 (2005).43E. R. Brown, K. A. McIntosh, K. B. Nichols, and C. L. Dennis, Appl.

Phys. Lett. 66, 285 (1995).44A. Shahvarpour, A. �Alvarez Melc�on, and C. Caloz, IEEE Trans. Antennas

Propag. 61, 4013 (2013).45H. Hu, F. Zhai, D. Hu, Z. Li, B. Bai, X. Yang, and Q. Dai, Nanoscale 7,

19493 (2015).46J. B. Khurgin, Nat. Nanotechnol. 10, 2 (2015).47D. F. Sievenpiper, “High-impedance electromagnetic surfaces,” Ph.D. the-

sis, Institution is University of California Los Angeles, 1999.

013103-10 Chu et al. J. Appl. Phys. 120, 013103 (2016)

00:47:32